Chem. Rev. 2010, 110, 3479–3500
Cellulose Nanocrystals: Chemistry, Self-Assembly, and Applications Youssef Habibi,† Lucian A. Lucia,*,† and Orlando J. Rojas†,‡ Department of Forest Biomaterials, North Carolina State University, Box 8005, Raleigh, North Carolina 27695-8005, and Department of Forest Products Technology, Faculty of Chemistry and Materials Sciences, Helsinki University of Technology, P.O. Box 3320, FIN-02015 TKK, Espoo, Finland Received October 12, 2009
Contents 1. Introduction and State of the Art 2. Structure and Morphology of Celluloses 3. Cellulose Nanocrystals 3.1. Preparation of Cellulose Nanocrystals 3.2. Morphology and Dimensions of Cellulose Nanocrystals 4. Chemical Modifications of Cellulose Nanocrystals 4.1. Noncovalent Surface Chemical Modifications 4.2. TEMPO-Mediated Oxidation 4.3. Cationization 4.4. Esterification, Silylation and Other Surface Chemical Modifications 4.5. Polymer Grafting 5. Self-Assembly and -Organization of Cellulose Nanocrystals 5.1. Self-Assembly and -Organization of CNs in Aqueous Medium 5.2. Self-Assembly and -Organization of CNs in Organic Medium 5.3. Self-Assembly and -Organization of CNs under External Fields 5.4. Self-Assembly and -Organization of CNs in Thin Solid Films 6. Applications of Cellulose Nanocrystals in Nanocomposite Materials 6.1. Nanocomposite Processing 6.1.1. Casting-Evaporation Processing 6.1.2. Sol-Gel Processing 6.1.3. Other Processing Methods 6.2. Mechanical Properties of CN-Based Composites 6.2.1. Morphology and Dimensions of CNs 6.2.2. Processing Method 6.2.3. Interfacial Interactions 6.3. Thermal Properties of CN-Based Composites 7. Conclusions and Outlook 8. Acknowledgments 9. References
3479 3480 3483 3483 3485 3486 3486 3487 3487 3487 3488 3489 3490 3492 3492 3492 3493 3493 3493 3494 3494 3495 3496 3496 3496 3496 3497 3497 3497
1. Introduction and State of the Art Cellulose constitutes the most abundant renewable polymer resource available today. As a chemical raw material, it is generally well-known that it has been used in the form of † ‡
North Carolina State University. Helsinki University of Technology.
Dr. Youssef Habibi is a research assistant professor at the Department of Forest Biomaterials at North Carolina State University. He received his Ph.D. in 2004 in organic chemistry from Joseph Fourier University (Grenoble, France) jointly with CERMAV (Centre de Recherche sur les Macromole´cules Ve´ge´tales) and Cadi Ayyad University (Marrakesh, Morocco). During his Ph.D., he worked on the structural characterization of cell wall polysaccharides and also performed surface chemical modification, mainly TEMPO-mediated oxidation, of crystalline polysaccharides, as well as their nanocrystals. Prior to joining NCSU, he worked as assistant professor at the French Engineering School of Paper, Printing and Biomaterials (PAGORA, Grenoble Institute of Technology, France) on the development of biodegradable nanocomposites based on nanocrystalline polysaccharides. He also spent two years as postdoctoral fellow at the French Institute for Agricultural Research, INRA, where he developed new nanostructured thin films based on cellulose nanowiskers. Dr. Habibi’s research interests include the sustainable production of materials from biomass, development of high performance nanocomposites from lignocellulosic materials, biomass conversion technologies, and the application of novel analytical tools in biomass research.
fibers or derivatives for nearly 150 years for a wide spectrum of products and materials in daily life. What has not been known until relatively recently is that when cellulose fibers are subjected to acid hydrolysis, the fibers yield defect-free, rod-like crystalline residues. Cellulose nanocrystals (CNs) have garnered in the materials community a tremendous level of attention that does not appear to be relenting. These biopolymeric assemblies warrant such attention not only because of their unsurpassed quintessential physical and chemical properties (as will become evident in the review) but also because of their inherent renewability and sustainability in addition to their abundance. They have been the subject of a wide array of research efforts as reinforcing agents in nanocomposites due to their low cost, availability, renewability, light weight, nanoscale dimension, and unique morphology. Indeed, CNs are the fundamental constitutive polymeric motifs of macroscopic cellulosic-based fibers whose sheer volume dwarfs any known natural or synthetic biomaterial. Biopolymers such as cellulose and lignin and
10.1021/cr900339w 2010 American Chemical Society Published on Web 03/04/2010
3480 Chemical Reviews, 2010, Vol. 110, No. 6
Dr. Lucian A. Lucia is currently an associate professor who works in the area of renewable materials chemistry and engineering in the Department of Forest Biomaterials (formerly Wood & Paper Science) at North Carolina State University. He received his Ph.D. in 1996 under Prof. Kirk S. Schanze from the University of Florida (Gainesville, FL) in organic chemistry with a focus on modeling the fundamental electron transfer pathways active in plant photosynthesis. He then spent almost 2 years at the NSF Center for Photoinduced Charge Transfer at the University of Rochester (Rochester, NY, under Prof. David G. Whitten) where he explored the design of highly functional materials based on photoactive amphiphiles and their behavior in heterogeneous media. He began his independent academic career as an assistant professor at the Institute of Paper Science and Technology at the Georgia Institute of Technology (Atlanta, GA) in 1997 where he extensively studied the materials chemistry and photochemistry of wood biopolymers. He joined the faculty at North Carolina State University in 2004 where he began to explore fundamental and applied aspects of renewable material-based composites. His research interests include antibacterial materials, cellulose nanocrystal templates, scaffolds for tissue engineering, drug delivery devices, biomass pretreatments, and wood pulping chemistry.
in some cases heteropolysaccharides provide the hierarchical constructs to bioengineer biological factories that give rise to a variegated distribution of plants and organisms. Surprisingly, a focus on nanoscale phenomena involving these materials has not been realized until the past few years in which a virtual collection of information has become available. In the following review, the salient chemical and physical features of the most dominant fundamental building block in the biosphere, cellulose nanocrystals, are discussed. After a brief introduction to cellulose, three general aspects of CNs are covered, namely, their morphology and chemistry including their preparation and chemical routes for functionalization, self-assembly in different media and under different conditions, and finally their applications in the nanocomposites field. While these aspects are by no means comprehensively inclusive of the vast number of research results available, they may be regarded as perhaps the most scientifically and technologically pertinent aspects of CNs that deserve attention.
2. Structure and Morphology of Celluloses Cellulose is the most abundant renewable organic material produced in the biosphere, having an annual production that is estimated to be over 7.5 × 1010 tons.1 Cellulose is widely distributed in higher plants, in several marine animals (for example, tunicates), and to a lesser degree in algae, fungi, bacteria, invertebrates, and even amoeba (protozoa), for example, Dictyostelium discoideum. In general, cellulose is a fibrous, tough, water-insoluble substance that plays an essential role in maintaining the structure of plant cell walls.
Habibi et al.
Dr. Orlando Rojas is Associate Professor in North Carolina State University and Finland Distinguished Professor in Helsinki University of Technology. He worked as a Senior Scientist in the Department of Chemistry, Physical Chemistry of the Royal Institute of Technology, KTH, and in the Institute for Surface Chemistry, YKI. Prior appointments include his tenure as professor in the Department of Chemical Engineering of Universidad de Los Andes (Venezuela), after obtaining his Ph.D. in Chemical Engineering in Auburn University and other graduate degrees that included a Diploma in Paper Engineering from the ETSII of Universidad Politecnica de Catalun˜a (Spain). He leads the “Colloids and Interfaces” Group at NC State University with a research focus on surface and colloid chemistry and the adsorption behaviors of surfactants and polymers at solid/liquid interfaces. He has studied the viscoelasticity of adsorbed monolayers by surface laser light scattering, surface plasmon resonance, and quartz crystal microgravimetry methods. His work has also involved state-ofthe-art interferometric and bimorph surface force techniques, as well as atomic force microscopy, to unveil basic phenomena and interactions at the nanoscale. His group currently works on nanocellulose structures, the dynamics of lignocellulose degradation, biosensor development, and separation, derivatization, and use of natural polymers and surfactants. He is Associate Editor of the Journal of Surfactants and Detergents and member of the advisory committee of several other journals. Dr. Rojas is the 2009-2010 Chair of the Division of “Cellulose and Renewable Materials” of the American Chemical Society and is the recipient of the 2009 American Chemical Society Divisional service Award. He was appointed 2009-2014 Finland Distinguish Professor by Tekes, the Finnish Funding Agency for Technology and Innovation and the Academy of Finland.
It was first discovered and isolated by Anselme Payen in 1838,2 and since then, multiple physical and chemical aspects of cellulose have been extensively studied; indeed, discoveries are constantly being made with respect to its biosynthesis, assembly, and structural features that have inspired a number of research efforts among a broad number of disciplines. Several reviews have already been published reporting the state of knowledge of this fascinating polymer.1,3-13 Regardless of its source, cellulose can be characterized as a high molecular weight homopolymer of β-1,4-linked anhydro-D-glucose units in which every unit is corkscrewed 180° with respect to its neighbors, and the repeat segment is frequently taken to be a dimer of glucose, known as cellobiose (Figure 1). Each cellulose chain possesses a directional chemical asymmetry with respect to the termini of its molecular axis: one end is a chemically reducing functionality (i.e., a hemiacetal unit) and the other has a pendant hydroxyl group, the nominal nonreducing end. The number of glucose units or the degree of polymerization (DP) is up to 20 000, but shorter cellulose chains can occur and are mainly localized in the primary cell walls. All β-D-glucopyranose rings adopt a 4C1 chair conformation, and as a consequence, the hydroxyl groups are positioned in the ring (equatorial) plane, while the hydrogen atoms are in the vertical position (axial). This structure is
Chemical Reviews, 2010, Vol. 110, No. 6 3481
Figure 1. Chemical structure of cellulose.
Figure 2. Intramolecular hydrogen-bonding network in a representative cellulose structure.
stabilized by an intramolecular hydrogen bond network extending from the O(3′)-H hydroxyl to the O(5) ring oxygen of the next unit across the glycosidic linkage and from the O(2)-H hydroxyl to the O(6′) hydroxyl of the next residue (Figure 2). The three most probable rotational positions of the hydroxymethyl group are defined by ascertaining the placement of the O6-C6 bond with respect to the O5-C5 and C4-C5 bonds: if O6-C6 is gauche to O5-C5 and trans to C4-C5, then the conformation is called gt, while the other two conformations are referred to as gg and tg (Figure 3). In nature, cellulose does not occur as an isolated individual molecule, but it is found as assemblies of individual cellulose chain-forming fibers. This is because cellulose is synthesized as individual molecules, which undergo spinning in a hierarchical order at the site of biosynthesis. Typically, approximately 36 individual cellulose molecules assemble are brought together into larger units known as elementary fibrils (protofibrils), which pack into larger units called microfibrils, and these are in turn assembled into the familiar cellulose fibers. However, celluloses from different sources may occur in different packing as dictated by the biosynthesis conditions. The combined actions of biopolymerization, spinning, and crystallization occur in a rosette-shaped plasma membrane complex having a diameter of 30 nm (Figure 4) and are orchestrated by specific enzymatic terminal complexes (TCs) that act as biological spinnerets.14 Because all the cellulose chains in one microfibril must be elongated by the complex at the same rate, crystallization during cellulose synthesis follows very closely polymerization of the chains by the TCs.15,16 TCs are thought to be cellulose synthase complexes that belong to the large GT-A family of glycosyltransferases; however, the reaction mechanism involved in cellulose synthesis and assembly is still conjectural. The
Figure 4. Orientation of microtubules controlling the orientation of cellulose in the cell wall where the microtubules act like tracks to guide the cellulose enzymes floating in the cell membrane. Reprinted with permission from Ref 17. Copyright 2002 Elsevier.
structure of cellulose microfibrils implies that their syntheses and assembly involve the coordinate activity of approximately 36 active sites.17 However, diverse cellulose structures in various organisms imply that the enzyme complex is modular.14,18 Recent evidence from live-cell imaging of cellulose indicates that microtubules exert a direct effect on the orientation of cellulose deposition under specific conditions, but microtubules are not required for oriented deposition of cellulose under other conditions (Figure 4). During the biosynthesis, cellulose chains are aggregated in microfibrils that display cross dimensions ranging from 2 to 20 nm, depending on the source of celluloses. The aggregation phenomenon occurs primarily via van der Waals forces and both intra- (Figure 2) and inter-molecular hydrogen bonds. If the TCs are not perturbed, they can generate a limitless supply of microfibrils having only a limited number of defects or amorphous domains.14,18 A number of models for the microfibril hierarchy have been proposed that attempt to describe the supramolecular structure of cellulose, including the crystalline structure, crystallite dimensions and defects, structural indices of amorphous domains, dimensions of fibrillar formation, etc. These models differ mainly in the description of the organization and the distribution of the amorphous or less ordered regions within the microfibril. After many years of controversy, it is common practice to acknowledge that the amorphous regions are distributed as chain dislocations on segments along the
Figure 3. The three most probable rotational positions of the hydroxymethyl group.
3482 Chemical Reviews, 2010, Vol. 110, No. 6
Figure 5. Schematic representation of the elementary fibril illustrating the microstructure of the elementary fibril and straindistorted regions (defects). Reprinted with permission from Ref 19. Copyright 1972 John Wiley and Sons.
elementary fibril where the microfibrils are distorted by internal strain in the fiber and proceed to tilt and twist (Figure 5).19 In the ordered regions, cellulose chains are tightly packed together in crystallites, which are stabilized by a strong and very complex intra- and intermolecular hydrogen-bond network. The hydrogen-bonding network and molecular orientation in cellulose can vary widely, which can give rise to cellulose polymorphs or allomorphs, depending on the respective source, method of extraction, or treament.1,20 Six interconvertible polymorphs of cellulose, namely, I, II, IIII, IIIII, IVI, and IVII, have been identified. Native cellulose has been thought to have one crystal structure, cellulose I, but evidence for the existence of two suballomorphs of cellulose I, termed IR and Iβ, was
Habibi et al.
established in 1984 by cross-polarization magic angle spinning (CP-MAS).21,22 Depending on the origin of cellulose, these two polymorphs exist in different ratios: IR is prevalent in celluloses from algae and bacteria, and both IR and Iβ may be present in celluloses in higher plants. However, the latter result is not without controversy. Solid-state NMR studies reported by Atalla and VanderHart23 has demonstrated several anomalies within the spectra of higher plant celluloses compared with those from algae, bacteria, and tunicates. The anomalies found in the NMR spectra seem to suggest that higher plants may contain only cellulose Iβ, instead of cellulose IR, with a distorted form of Iβ that resides below the surface. In both the Iβ and IR structures, cellulose chains adopt parallel configurations, but they differ in their hydrogenbonding patterns, which implies a difference in the crystalline structure (Figure 6). Indeed, IR corresponds to a triclinic P1 unit cell (a ) 6.717 Å, b ) 5.962 Å, c ) 10.400 Å, R ) 118.08°, β ) 114.80°, and γ ) 80.37°) containing only one chain per unit cell,24 whereas Iβ exists in a monoclinic P21 unit cell having two cellulose chains (a ) 7.784 Å, b ) 8.201 Å, c ) 10.38 Å, R ) β ) 90°, and γ ) 96.5°).25 IR, a metastable phase, can be converted to the more thermodynamically stable Iβ phase by high-temperature annealing in various media.26 Cellulose I (R and β) has sheets stacked in a “parallel-up” fashion, and the hydroxylmethyl groups are oriented in a tg conformation so that their O6 atom points toward the O2 hydroxyl groups of the neighboring residue, which engenders a second inter-residue hydrogen bond.27 If cellulose is bent in a plane orthogonal to the hydrogenbonded sheets of chains, a horizontal displacement of the sheets with respect to one another is induced.28 A bending angle of 39° has been shown to be sufficient to induce IR and Iβ interconversion especially when the curvature of the chain sheets in the microfibril is modeled as a group of concentric circular arcs. Sine qua non, all microfibrils
Figure 6. Hydrogen-bonding patterns in cellulose IR and Iβ: (top) the two alternative hydrogen-bond networks in cellulose IR; (bottom) the dominant hydrogen-bond network in cellulose Iβ (left) chains at the origin of the unit cell and (right) chains at the center of the unit cell according to Sturcova et al.32 Reprinted with permission from ref 32. Copyright 2004 American Chemical Society.
generated from the TCs must torque sharply before they can adopt a parallel configuration with respect to the face of the inner cell wall. Therefore, the crystal form is likely to be drastically changed before cellulose is incorporated into the cell wall. Such polymorphic differences were first evidenced by IR spectroscopy29 and electron diffraction30 and have been further confirmed more recently by solid-state CP/MAS 13C NMR.21 The crystal structure and hydrogen-bonding pattern of cellulose I (R and β) were later studied more deeply by synchrotron X-ray and neutron fiber diffraction,24,25,31 where in the latter, the hydrogen atom positions involved in hydrogen bonding were determined from Fourier-difference analysis with respect to hydrogenated and deuterated samples. The definition of all atomic spatial coordinates in the cellulose crystal structure was only possible for the first time because of the availability of these singular methods. Cellulose II, the second most extensively studied allomorph, can be obtained by two different processes: (i) By chemical regeneration, which consists of dissolving cellulose I in a solvent, then reprecipitating it in water. Suitable solvents for cellulose include, among others, solutions of heavy metal-amine complexes, mainly copper with ammonia or diamine such as cupric hydroxide in aqueous ammonia (Scheweizer’s reagent called cuoxam)33 or cupriethylenediamine (cuen),34 ammonia or amine/thiocyanate,35 hydrazine/thiocyanate,36 lithium chloride/N,N-dimethylacetamide (LiCl/DMAc),37,38 and N-methylmorpholine-N-oxide (NMMO)/water39-41 systems. (ii) By mercerization, a universally recognized process the name of which is derived from its inventor John Mercer (1844),42 which consists of swelling native cellulose in concentrated sodium hydroxide solutions and yielding cellulose II after removing the swelling agent. Other swelling agents, such as nitric acid (65%), are also able to convert native fibers to cellulose II.43 Some atypical bacterial species are reported to biosynthesize cellulose II.44 Cellulose II exists in a monoclinic P21 phase (a ) 8.10 Å, b ) 9.03 Å, c ) 10.31 Å, R ) β ) 90°, and γ ) 117.10°).27,45,46 During conversion (I to II), the hydroxyl groups rotate from the tg to the gt conformation, which explicitly requires a change in the hydrogen-bond network.47,48 In contrast to cellulose I, which has a parallel up arrangement, the chains in cellulose II are in an antiparallel arrangement yielding a more stable structure, which makes it preferable for various textiles and paper materials. The conversion of cellulose I to cellulose II has been widely considered irreversible, although (partial) regeneration of cellulose I from cellulose II has been reported.49,50 If cellulose I or II is exposed to ammonia (gas or liquefied) or various amines,51 cellulose III is formed upon removal of the swelling agent. The resulting form of cellulose III depends on whether the starting form is I or II, giving rise to cellulose IIII or IIIII. Their diffraction patterns are similar except for the meridional intensities. Cellulose IIII exists in a monoclinic P21 form (a ) 4.450 Å, b ) 7.850 Å, c ) 10.31 Å, R ) β ) 90°, and γ ) 105.10°) with one chain in the unit cell, displaying parallel chains as observed in cellulose I.52 However, the hydroxymethyl groups are in the gt conformation and the intersheet hydrogen bond network is similar to cellulose II. The exact structure of cellulose IIIII is not clearly established yet, but the crystallographic and spectroscopic studies reported recently by Wada et al.53
Chemical Reviews, 2010, Vol. 110, No. 6 3483
indicate that cellulose IIIII is a disordered phase of cellulose. This disordered structure mainly contains a crystalline form having a unit cell (space group P21; a ) 4.45 Å, b ) 7.64 Å, c ) 10.36 Å, R ) β ) 90°, γ ) 106.96°) occupied by one chain organized in antiparallel fashion, in addition to a second structure, as revealed by CP/MAS 13C NMR (space group P21; a ) 4.45 Å, b ) 14.64 Å, c ) 10.36 Å, R ) β ) 90°, γ ) 90.05°). Furthermore, either of these forms IIII or IIIII reverts to its parent structure if placed in a hightemperature and humid environment. Polymorphs IVI and IVII may be prepared by heating cellulose IIII or IIIII, respectively, up to 260 °C in glycerol.54,55 In a like manner to the case of cellulose III, these two forms can revert to the parent structures I or II. In addition to the native cellulose I, it has been shown that cellulose IV exists in several plant primary cell walls.56,57
3. Cellulose Nanocrystals In the 1950s, Ra¨nby reported for the first time that colloidal suspensions of cellulose can be obtained by controlled sulfuric acid-catalyzed degradation of cellulose fibers.58-60 This work was inspired by the studies of Nickerson and Habrle61 who observed that the degradation induced by boiling cellulose fibers in acidic solution reached a limit after a certain time of treatment. Transmission electron microscopy (TEM) images of dried suspensions revealed for the first time the presence of aggregates of needle-shaped particles, while further analyses of these rods with electron diffraction demonstrated that they had the same crystalline structure as the original fibers.62,63 Simultaneously, the development by Battista64,65 of the hydrochloric acid-assisted degradation of cellulose fibers derived from high-quality wood pulps, followed by sonification treatment, led to the commercialization of microcrystalline cellulose (MCC). Stable, chemically inactive, and physiologically inert with attractive binding properties, MCC offered a significant opportunity for multiple uses in pharmaceutical industry as a tablet binder, in food applications as a texturizing agent and fat replacer, and also, as an additive in paper and composites applications. After the acid hydrolysis conditions were optimized, Marchessault et al.66 demonstrated that colloidal suspensions of cellulose nanocrystals exhibited nematic liquid crystalline alignment. Since the discovery of spectacular improvements in the mechanical properties of nanocomposites with cellulose nanocrystals,67,68 substantial research has been directed to cellulose nanocrystal composites because of the growing interest in fabricating materials from renewable resources. Cellulose nanocrystals are often referred to as microcrystals, whiskers, nanocrystals, nanoparticles, microcrystallites, or nanofibers. Hereafter, they are called “cellulose nanocrystals” (CNs). In the coming sections, methods for separation of CNs and their morphologies, characterization, modification, self-assembly, and applications will be reviewed.
3.1. Preparation of Cellulose Nanocrystals The main process for the isolation of CNs from cellulose fibers is based on acid hydrolysis. Disordered or paracrystalline regions of cellulose are preferentially hydrolyzed, whereas crystalline regions that have a higher resistance to acid attack remain intact.69,70 Thus, following an acid treatment that hydrolyzes the cellulose (leading to removal of the microfibrils at the defects), cellulose rod-like nanocrystals are produced. The obtained CNs have a morphology
3484 Chemical Reviews, 2010, Vol. 110, No. 6
Figure 7. TEM images of dried dispersion of cellulose nanocrystals derived from (a) tunicate79 (Reprinted with permission from ref 79. Copyright 2008 American Chemical Society), (b) bacterial80 (Reprinted with permission from ref 80. Copyright 2004 American Chemical Society), (c) ramie81 (From ref 81, Reproduced by permission of The Royal Society of Chemistry), and (d) sisal82 (Reprinted with permission from ref 82. Copyright 2006 Springer).
and crystallinity similar to the original cellulose fibers; examples of such elements are given in Figure 7. The actual occurrence of the acid cleavage event is attributed to differences in the kinetics of hydrolysis between amorphous and crystalline domains. In general, acid hydrolysis of native cellulose induces a rapid decrease in its degree of polymerization (DP), to the so-called level-off DP (LODP). The DP subsequently decreases much more slowly, even during prolonged hydrolysis times.65,71-75 LODP has been thought to correlate with crystal sizes along the longitudinal direction of cellulose chains present in the original cellulose before the acid hydrolysis. This hypothesis was based on the reasonable assumption that disordered or para-crystalline domains are regularly distributed along the microfibers and therefore they are more susceptible to acid attack (in contrast to crystalline regions that are more impervious to attack). Also, homogeneous crystallites were supposed to be generated after acid hydrolysis. These assumptions were actually confirmed by X-ray crystal diffraction,76 electron microscopy with iodine-staining,76 small-angle X-ray diffraction,72 and neutron diffraction analyses.77 It was shown that the LODP values obtained by acid hydrolysis of cellulose correlated well with the periodic crystal sizes along cellulose chains. The value of LODP has been shown to depend on the cellulose origin, with typical values of 250 being recorded for hydrolyzed cotton,64 300 for ramie fibers,77 140-200 for bleached wood pulp,65 and up to 6000 for the highly crystalline Valonia cellulose.78 However, a wide distribution of DPs is typically observed for different cellulose sources, even at the LODP. Such a disparity in the quoted distributions stimulates vigorous discussion to the present day. In fact, the acid hydrolysis of bacterial, tunicate, Valonia, or cotton results in a higher polydispersity in the molecular weight, without any evidence of the LODP, probably because these cellulosic materials have no regular distribution of the less-organized domains. Typical procedures currently employed for the production of CNs consist of subjecting pure cellulosic material to strong acid hydrolysis under strictly controlled conditions of tem-
Habibi et al.
perature, agitation, and time. The nature of the acid and the acid-to-cellulosic fibers ratio are also important parameters that affect the preparation of CNs. A resulting suspension is subsequently diluted with water and washed with successive centrifugations. Dialysis against distilled water is then performed to remove any free acid molecules from the dispersion. Additional steps such as filtration,79 differential centrifugation,83 or ultracentrifugation (using a saccharose gradient)84 have been also reported. Specific hydrolysis and separation protocols have been developed that depend on the origin of the cellulosic fibers. Most common sources include among others, cellulose fibers from cotton,85,86 ramie,81,87,88 hemp,89 flax,90,91 sisal,82,92 wheat straw,93 palm,94 bleached softwood95 and hardwood96 pulps, cotton linters pulp,97,98 microcrystalline cellulose,99-102 sugar beet pulp,103 bacterial cellulose,104-106 and Tunicates.69,84,107 Sulfuric and hydrochloric acids have been extensively used for CN preparation, but phosphoric108-111 and hydrobromic112 acids have also been reported for such purposes. If the CNs are prepared by hydrolysis in hydrochloric acid, their ability to disperse is limited and their aqueous suspensions tend to flocculate.113 On the other hand, when sulfuric acid is used as a hydrolyzing agent, it reacts with the surface hydroxyl groups of cellulose to yield charged surface sulfate esters that promote dispersion of the CNs in water, resulting in important properties that will be discussed shortly.114 However, the introduction of charged sulfate groups compromises the thermostability of the nanocrystals.80 Also, differences in the rheological behavior have been shown between suspensions obtained from sulfuric acid hydrolysis and those obtained from hydrochloric acid. In fact, the sulfuric acidtreated suspension has shown no time-dependent viscosity, whereas the hydrochloric acid-treated suspension showed a thixotropic behavior at concentrations above 0.5% (w/v) and antithixotropic behavior at concentrations below 0.3%.113 Post-treatment of CNs generated by hydrochloric acid hydrolysis with sulfuric acid has been studied to introduce, in a controlled fashion, sulfate moieties on their surfaces.86,95 CNs generated from hydrochloric acid hydrolysis and then treated with sulfuric acid solution had the same particle size as those directly obtained from sulfuric acid hydrolysis; however, the surface charge density could be tuned to given values by sulfuric acid hydrolysis. With respect to the morphology of the particles, a combination of both sulfuric and hydrochloric acids during hydrolysis steps appears to generate spherical CNs instead of rod-like nanocrystals when carried out under ultrasonic treatment.115,116 These spherical CNs demonstrated better thermal stability mainly because they possess fewer sulfate groups on their surfaces.116 The concentration of sulfuric acid in hydrolysis reactions to obtain CNs does not vary much from a typical value of ca. 65% (wt); however, the temperature can range from room temperature up to 70 °C and the corresponding hydrolysis time can be varied from 30 min to overnight depending on the temperature. In the case of hydrochloric acid-catalyzed hydrolysis, the reaction is usually carried out at reflux temperature and an acid concentration between 2.5 and 4 N with variable time of reaction depending on the source of the cellulosic material. Bondenson et al.99,102 investigated optimizing the hydrolysis conditions by an experimental factorial design matrix (response surface methodology) using MCC that was derived from Norway spruce (Picea abies) as the cellulosic starting material. The factors that were varied during the process were the concentrations of MCC and
sulfuric acid, the hydrolysis time and temperature, and the ultrasonic treatment time. The responses that were measured were the median size of the cellulose particles and the yield of the reaction. The authors demonstrated that with a sulfuric acid concentration of 63.5% (w/w) over a time of approximately 2 h, it was possible to obtain CNs having a length between 200 and 400 nm and a width less than 10 nm with a yield of 30% (based on initial weight). Prolongation of the hydrolysis time induced a decrease in nanocrystal length and an increase in surface charge.85 Reaction time and acid-to-pulp ratio on nanocrystals obtained by sulfuric acid hydrolysis of bleached softwood (black spruce, Picea mariana) sulfite pulp was investigated by Beck-Candanedo et al.96 They reported that shorter nanoparticles with narrow size polydispersity were produced at longer hydrolysis times. Recently, Elazzouzi-Hafraoui et al.79 studied the size distribution of CNs resulting from sulfuric acid hydrolysis of cotton treated with 65% sulfuric acid over 30 min at different temperatures, ranging from 45 to 72 °C. By increasing the temperature, they demonstrated that shorter crystals were obtained; however, no clear influence on the width of the crystal was revealed.
3.2. Morphology and Dimensions of Cellulose Nanocrystals The geometrical dimensions (length, L, and width, w) of CNs are found to vary widely, depending on the source of the cellulosic material and the conditions under which the hydrolysis is performed. Such variations are due, in part, to the diffusioncontrolled nature of the acid hydrolysis. The heterogeneity in size in CNs obtained from hydrolysis, for a given source type, can be reduced by incorporating filtration,79 differential centrifugation,83 or ultracentrifugation (using a saccharose gradient)84 steps. The precise morphological characteristics are usually studied by microscopy (TEM, AFM, E-SEM,117 etc.) or light scattering techniques, including small angle neutron scattering (SANS)118 and polarized and depolarized dynamic light scattering (DLS, DDLS).119 TEM images of CNs typically show aggregation of the particles, mainly due to the drying step for the preparation of the specimens after negative staining. Besides aggregation, additional instrumental artifacts usually lead to an overestimation of CN dimensions. To overcome these issues, Elazzouzi-Hafraoui et al.79 recently reported the use of TEM in cryogenic mode (cryo-TEM) to prevent aggregation. Atomic force microscopy (AFM) has been widely used to provide valuable and rapid indication of surface topography of CNs under ambient conditions at length scales down to the a˚ngstro¨m level.117,120-122 However, AFM topography may show rounded cross-sectional profiles in cases where other shapes are expected; for example, AFM imaging of Valonia gives shapes different than the square shape cross section observed under TEM. This is probably due to artifacts that result from substrate shape perturbations induced by AFM tip and tip-broadening effects. Finally, AFM was also reported to be a valuable technique to measure CNs mechanical properties and interactions, such as stiffness and adhesion or pull-off forces.123 Typical geometrical characteristics for CNs originating from different cellulose sources and obtained with a variety of techniques are summarized in Table 1. The reported width is generally approximately a few nanometers, but the length of CNs spans a larger window, from tens of nanometers to several micrometers. An arresting observation is that there
Chemical Reviews, 2010, Vol. 110, No. 6 3485 Table 1. Examples of the Length (L) and Width (w) of CNs from Various Sources Obtained by Different Techniques source bacterial cotton
cotton linter MCC ramie sisal
100-1000 100-1000 100-150 70-170 200-300 255 150-210 100-200 25-320 300-500 35-265 250-270 ∼500 150-250 50-150 100-500 150-280
10-50 5-10 × 30-50 5-10 ∼7 8 15 5-11 10-20 6-70 15-30 3-48 23 10 6-8 5-10 3-5 3.5-6.5 8.8 × 18.2 16 10 15-30 15 28 10-20 3-4 4-5 4-5
TEM TEM TEM TEM TEM DDL AFM SEM-FEG TEM AFM TEM TEM AFM TEM TEM TEM TEM SANS DDL TEM TEM TEM TEM TEM TEM AFM AFM
105 80, 104 127 128 129 119 117 97 79 130 79 101 100 81 131 82 92 118 119 107 132 129 79 125 95, 113 96 96
Valonia soft wood hard wood
1160 500-1000 1000-3000 100-1000 1073 >1000 100-200 100-150 140-150
is a direct correspondence between the length of the CNs and the LODP of the corresponding material because it is generally recognized that the rodlike CN consists of fully extended cellulose chain segments in a perfectly crystalline arrangement. CNs from wood are 3-5 nm in width and 100-200 nm in length, while those for Valonia, a sea plant, are reported to be 20 nm in width and 1000-2000 nm in length. Likewise, cotton gives CNs 5-10 nm in width and 100-300 nm long, and tunicate, a sea animal, gives ca. 10-20 nm in width and 500-2000 nm long.69 The aspect ratio, defined as the length-to-width (L/w) spans a broad range and can vary between 10 and 30 for cotton and ca. 70 for tunicate. The morphology of the cross section of CNs also depends on the origin of the cellulose fibers. The basis of the morphological shape in the cross section may be attributed to the action of the terminal complexes during cellulose biosynthesis. In fact, depending on the biological origin of the cell wall, different arrangements of TCs have been observed, which generate cellulose crystals with different geometries.14 Despite the fact that acid hydrolysis appears to erode the crystal by preferentially peeling off angular cellulose sheets, as has been reported by Helbert et al.,124 a number of analyses of cross sections of CNs have nevertheless attempted to characterize the inherent CN geometry. Based on TEM observations, Revol125 reported that the cross section of cellulose crystallites in Valonia Ventricosa was almost square, with an average lateral element length of 18 nm. In contrast, CNs from tunicate that were analyzed by TEM126 and SANS were found to have a rectangular 8.8 nm × 18.2 nm cross-sectional shape.118 The morphology of CNs along the axis of the crystal seems to also present different features, depending on the source of the nanocrystal. CNs from bacterial cellulose121 and tunicate79 have been reported to have ribbon-like shapes with twists having half-helical pitches of 600-800 nm (Micrasterias denticulata) and 1.2-1.6 µm, respectively. However,
3486 Chemical Reviews, 2010, Vol. 110, No. 6
these twisted features have not been clearly evidenced in CNs extracted from higher plants, which are believed to be flat with uniplanar-axial orientation.
4. Chemical Modifications of Cellulose Nanocrystals Because of a natural advantage of an abundance of hydroxyl groups at the surface of CNs, different chemical modifications have been attempted, including esterification, etherification, oxidation, silylation, polymer grafting, etc. Noncovalent surface modification, including the use of adsorbing surfactants and polymer coating, has been also studied. All chemical functionalizations have been mainly conducted to (1) introduce stable negative or positive electrostatic charges on the surface of CNs to obtain better dispersion (CNs obtained after sulfuric acid hydrolysis introduce labile sulfate moieties that are readily removed
Habibi et al.
under mild alkaline conditions) and (2) tune the surface energy characteristics of CNs to improve compatibility, especially when used in conjunction with nonpolar or hydrophobic matrices in nanocomposites. The main challenge for the chemical functionalization of CNs is to conduct the process in such a way that it only changes the surface of CNs, while preserving the original morphology to avoid any polymorphic conversion and to maintain the integrity of the crystal.
4.1. Noncovalent Surface Chemical Modifications Noncovalent surface modifications of CNs are typically made via adsorption of surfactants. This approach has been introduced by Heux et al.,129,133 who used surfactants consisting of the mono- and di-esters of phosphoric acid bearing alkylphenol tails. The obtained surfactant-coated CNs dispersed very well in nonpolar solvents.129 Detailed analyses
Figure 8. Scheme of TEMPO-mediated oxidation mechanism of the hydroxymethyl groups of cellulose (top, reaction scheme) and crosssectional representation of cellulose nanocrystal indicating the occurrence of the surface TEMPO-mediated oxidation of available hydroxyl groups (bottom, surface crystal representations).
Chemical Reviews, 2010, Vol. 110, No. 6 3487
of the data provided by SANS revealed that the surfactant molecules formed a thin layer of about 15 Å at the surface of the CNs.134 When the surface-modified CNs were incorporated into isotactic polypropylene, they showed very good compatibility and they acted as remarkable nucleating agents to induce the formation of the rare β crystalline form in addition to the regular crystalline form of isotactic polypropylene R.135,136 An anionic surfactant was also used by Bondeson et al.137 to enhance the dispersion of CNs in poly(lactic acid) (PLA). Kim et al.138 and Rojas et al.139 used nonionic surfactants to disperse CNs in polystyrene-based composite fibers. Zhou et al.140 recently reported a new and elegant way of CN surface modification based on the adsorption of saccharide-based amphiphilic block copolymers. By mimicking lignin-carbohydrate copolymers, they adsorbed xyloglucan oligosaccharide-poly(ethylene glycol)polystyrene triblock copolymer onto the surface of CNs. The resulting CNs showed excellent dispersion abilities in nonpolar solvents.
4.2. TEMPO-Mediated Oxidation (2,2,6,6-Tetramethylpiperidine-1-oxyl)-mediated (or TEMPO-mediated) oxidation of CNs has been used to convert the hydroxylmethyl groups present on their surface to their carboxylic form. This oxidation reaction, which is highly discriminative of primary hydroxyl groups, is also “green” and simple to implement. It involves the application of a stable nitroxyl radical, the 2,2,6,6tetramethylpiperidine-1-oxyl (TEMPO), in the presence of NaBr and NaOCl (see Figure 8, top). The use of this technique has been the subject of a number of reports since it was first introduced by De Nooy et al.,141 who showed that only the hydroxymethyl groups of polysaccharides were oxidized, while the secondary hydroxyls remained unaffected. In fact, TEMPO-mediated oxidation of CNs involves a topologically confined reaction sequence, and as a consequence of the 2-fold screw axis of the cellulose chain, only half of the accessible hydroxymethyl groups are available to react, whereas the other half are buried within the crystalline particle (Figure 8, bottom). TEMPO-mediated oxidation of CNs, obtained from HCl hydrolysis of cellulose fibers, was first reported by Araki et al.127 as an intermediate step to promote grafting of polymeric chains. These authors demonstrated that after TEMPOmediated oxidation, the CNs maintained their initial morphological integrity and formed a homogeneous suspension when dispersed in water. The basis for these latter observations was the presence of the newly installed carboxyl groups that imparted negative charges at the CN surface and thus induced electrostatic stabilization. Similar observations were reported by Montanari et al.142 who also showed that during excessive TEMPO-mediated oxidation, a decrease of the crystal size occurred resulting from the partial delamination of cellulose chains that are extant on the surface. Habibi et al.143 performed TEMPO-mediated oxidation of CNs obtained from HCl hydrolysis of cellulose fibers from tunicate and showed that it did not compromise the morphological integrity of CNs or their native crystallinity. On the basis of the supramolecular structure, morphology, and crystallographic parameters of the CNs, these authors demonstrated that various degrees of oxidation can be predicted and achieved by using specific amounts of the primary oxidizing agent, that is, NaOCl (see Figure 8, bottom). When dispersed in water, TEMPO-oxidized or
Figure 9. Aqueous 0.53% (w/v) suspensions of cellulose nanocrystals observed between crossed polarizers (1) after production by HCl-catalyzed hydrolysis (left) and (2) after their oxidation via TEMPO-mediated reactions (right). Reprinted with permission from ref 143. Copyright 2006 Springer.
carboxylated CN suspensions display birefringence patterns and do not flocculate or sediment owing to the polyanionic character imparted by the negative charges on the CNs surfaces (see Figure 9).
4.3. Cationization Positive charges can also be easily introduced on the surface of CNs; for example, weak or strong ammoniumcontaining groups, such as epoxypropyltrimethylammonium chloride (EPTMAC), can be grafted onto the CN surfaces.144 Such surface cationization proceeds via a nucleophilic addition of the alkali-activated cellulose hydroxyl groups to the epoxy moiety of EPTMAC and leads to stable aqueous suspensions of CNs with unexpected thixotropic gelling properties. Shear birefringence was observed, but no liquid crystalline chiral nematic phase separation was detected for these cationic CNs, most likely owing to the high viscosity of the suspension.
4.4. Esterification, Silylation and Other Surface Chemical Modifications Homogeneous and heterogeneous acetylation of model CNs extracted from Valonia and tunicate has been studied by Sassi and Chanzy by using acetic anhydride in acetic acid.126 Their ultrastructural study, carried out by TEM imaging and X-ray diffraction, showed that the reaction proceeded by a reduction of the diameters of the crystals, while only a limited reduction in CN length was observed. It has been suggested that the reaction involved a nonswelling mechanism that affected only the cellulose chains localized at the crystal surface. In the case of homogeneous acetylation, the partially acetylated molecules immediately partitioned into the acetylating medium as soon as they were sufficiently soluble, while in heterogeneous conditions, the cellulose acetate remained insoluble and surrounded the crystalline core of unreacted cellulose chains. The simultaneous occurrence of cellulose hydrolysis and acetylation of hydroxyl
3488 Chemical Reviews, 2010, Vol. 110, No. 6
Habibi et al.
Figure 10. Reaction scheme illustrating the one-pot (tandem) cellulose hydrolysis and esterification reactivity of hydroxyl groups. Reprinted with permission from ref 145. Copyright 2009 American Chemical Society.
groups has been also reported. Fischer esterification of hydroxyl groups simultaneously with the hydrolysis of amorphous cellulose chains has been introduced as a viable one-pot reaction methodology that allows isolation of acetylated CNs in a single-step process (Figure 10).145,146 An environmentally friendly CN surface acetylation route was recently developed by Yuan et al.147 involving a low reagent consumption and simple-to-apply procedure. The method used alkyenyl succinic anhydride (ASA) aqueous emulsions as a template. The emulsions were simply mixed with CN suspensions and freeze-dried, and the resulting solid was heated to 105 °C. The obtained derivative conferred to the acylated CNs a highly hydrophobic character that was evident because they were easily dispersible in solvents with widely different polarities as measured by the respective dielectric constant, ε; for example, they were dispersible not only in DMSO having a very high ε of 46.45 but also in 1,4-dioxane that has a quite low ε of 2.21. Berlioz et al.148 have reported recently a new and highly efficient synthetic method for an almost complete surface esterification of CNs, leading to highly substituted CN esters. The reaction of fatty acid chains was carried out on dried CNs via a gas-phase process. It has been shown by SEM and X-ray diffraction analyses that the esterification proceeded from the surface of the substrate to the crystal core. Under moderate conditions, the surface was fully reacted, whereas the original morphology was maintained and the core of the crystal remained unmodified. Esterification of CNs by reacting organic fatty acid chlorides, having different lengths of the aliphatic chain (C12 to C18), has also been reported with a grafting density high enough that the fatty acids with backbones of 18 carbons were able to crystallize on the surface of the CNs.131 Cellulose whiskers resulting from the acid hydrolysis of tunicate have been partially silylated by a series of alkyldimethylchlorosilanes, with the carbon backbone of the alkyl moieties ranging from a short carbon length of isopropyl to longer lengths represented by n-butyl, n-octyl, and ndodecyl.149 It has been demonstrated that with a degree of
substitution (DS) between 0.6 and 1, the whiskers became readily dispersible in solvents of low polarity (such as THF) leading to stable suspensions with birefringent behavior, while their morphological integrity was preserved. However, at high silylation (DS greater than 1), the chains in the core of the crystals became silylated, resulting in the disintegration of the crystals and consequently the loss of original morphology. Surface trimethyl silylation of CNs from bacterial cellulose and their resulting cellulose acetate butyrate104,150 or polysiloxane151 based nanocomposites was also investigated by Roman and Winter. Finally, coupling CNs with N-octadecyl isocyanate, via a bulk reaction in toluene, has also been reported to enhance their dispersion in organic medium and compatibility with polycaprolactone, which significantly improved the stiffness and ductility of the resultant nanocomposites.92
4.5. Polymer Grafting Polymer grafting on the surface of CNs has been carried out using two main strategies, namely, the “grafting-onto” and “grafting-from”.152 The grafting onto approach involves attachment onto hydroxyl groups at the cellulose surface of presynthesized polymer chains by using a coupling agent. In the “grafting from” approach, the polymer chains are formed by in situ surface-initiated polymerization from immobilized initiators on the substrate. The “grafting onto” approach was used by Ljungberg et al.153 to graft maleated polypropylene (PPgMA) onto the surface of tunicate-extracted CNs. The resulting grafted nanocrystals showed very good compatibility and high adhesion when dispersed in atactic polypropylene. Araki et al.127 and Vignon et al.154 studied the grafting of amineterminated polymers on the surface of TEMPO-mediated oxidized CNs by using a peptide coupling process catalyzed by carbodiimide derivatives in water. The same approach has been implemented by Mangalam et al.155 who grafted DNA oligomers on the surface of CNs. The grafting of polycaprolactone having different molecular weights on the
surface of CNs has been achieved by using isocyanatemediated coupling.87 These authors reported reaching a grafting density that was high enough that the grafted PCL chains were able to crystallize at the surface of CNs. Similar efforts were made by Cao et al.98 who reported the isocyanate-catalyzed grafting of presynthesized water-borne polyurethane polymers via a one-pot process. Such crystallization provoked cocrystallizations of the free chains of the respective polymer matrices during CN-based nanocomposite processing. Furthermore, this cocrystallization phenomenon induced the formation of a co-continuous phase between the matrix and filler, which significantly enhanced the interfacial adhesion and consequently contributed to a highly improved mechanical strength of the resulting nanocomposites. The “grafting from” approach applied to CNs was first reported by Habibi et al.,81 who grafted polycaprolactone onto the surface of CNs via ring-opening polymerization (ROP) using stannous octoate (Sn(Oct)2) as a grafting and polymerization agent. Likewise, Chen et al.156 and Lin et al.157 conducted similar grafting reactions under microwave irradiation to enhance the grafting efficiency. In situ polymerization of furfuryl alcohol from the surface of cellulose whiskers was studied by Pranger et al.100 In this case, the polymerization was catalyzed by sulfonic acid residues from the CN surface. At elevated temperatures, the sulfonic acid groups were de-esterified and consequently released into the medium to catalyze in situ the polymerization. Yi et al.158 and Morandi et al.159 propagated polystyrene brushes via atom transfer radical polymerization (ATRP) on the surface of CNs with ethyl 2-bromoisobutyrate as the initiator agent. Similarly, other vinyl monomers, mainly acrylic monomers such as N-isopropylacrylamide, were also polymerized from the surface of CNs to produce thermoresponsive substrates.160,161 Grafting of polyaniline from CNs was achieved by in situ polymerization of aniline onto CNs in hydrochloric acid aqueous solution, via an oxidative polymerization using ammonium peroxydisulfate as the initiator.162
5. Self-Assembly and -Organization of Cellulose Nanocrystals When sulfuric acid is used as the hydrolyzing agent, it also chemically reacts with the surface hydroxyl groups of CNs to yield negatively charged (surface) sulfate groups that promote a perfectly uniform dispersion of the whiskers in water via electrostatic repulsions.114 By inference, continuous
Chemical Reviews, 2010, Vol. 110, No. 6 3489
removal of the water phase should therefore tend to cause the nanocrystals to adopt configurations that minimize the existing electrostatic interactions. Indeed, (homogeneous) concentrated suspensions self-organize into spectacular liquid crystalline arrangements, a phenomenon similar to what occurs in nonflocculating suspensions of other rod-like particles, such as poly(tetrafluoroethylene) whiskers,163 tobacco mosaic viruses (TMV),164 DNA fragments,165 or crystallites extracted from other polysaccharides such as chitin.166 This self-organization phenomenon was revealed by the appearance of “fingerprint” patterns obtained from suspensions observed by polarized optical microscopy, indicative of a chiral-nematic ordering.114 An even more striking finding is that this chiral nematic structure can be preserved after complete water evaporation to provide iridescent films of CNs. These solid films, in addition to allowing fundamental studies of their striking behavior, have numerous potential applications such as coating materials for decorative materials and security papers (because the optical properties cannot be reproduced by printing or photocopying).167 An investigation into these systems reveals that CNs are randomly oriented in the dilute regime (isotropic phase). Indeed, polarized optical microscopy demonstrates that at dilute concentrations, CNs appear as spheroids or ovaloids and the initial ordered domains are similar to tactoids. A nematic liquid crystalline alignment is adopted when the CN concentration increases because these tactoids coalesce to form an anisotropic phase, which is characterized by a unidirectional self-orientation of the CN rods. When the suspension reaches a critical concentration of CNs, it forms a chiral nematic ordered phase displaying lines that are the signature of cholesteric liquid crystals (see Figure 14). Above the critical concentration of chiral nematic phase formation, aqueous CN suspensions produce shear birefringence, and on standing, they can spontaneously separate into an upper isotropic and a lower anisotropic phase (Figure 11). These chiral nematic or cholesteric structures in the anisotropic phase consist of stacked planes of CN rods aligned along a vector (director), with the orientation of each director rotated about the perpendicular axis from one plane to the next as shown in Figure 11. The self-induced parallel alignment phenomenon of the CNs that occurs above a critical concentration is attributed to the well-known entropically driven self-orientation phenomenon of rod-like
Figure 11. (left) Aqueous 0.63% (w/w) CN suspension observed between crossed polarizers. Immediately after shearing the suspension shows many iridescent birefringence patterns; after 1 week, the suspension separates into the upper isotropic and the lower anisotropic phases (Reprinted with permission from ref 105. Copyright 2001 American Chemical Society). (right) Schematic representation of CN orientation in both the isotropic and anisotropic (chiral nematic) phases.
3490 Chemical Reviews, 2010, Vol. 110, No. 6
Habibi et al.
Figure 12. (top) Representations suggested by Orts et al. for the tighter packing achievable by the chiral interaction of twisted rods: left, the distance between rods is reduced to D if instead of rods packing with axes parallel they pack with the “thread” of one rod fitting into the “groove” of its neighbor; (right) for nanocrystals with an electrostatic double layer, a threaded rod would alter the surrounding electric double layer and affect packing over relatively large distances (Reprinted with permission from ref 170. Copyright 1998 American Chemical Society). (bottom) Schematic illustration of bacterial cellulose nanocrocrystals with surface charge, showing the change in effective particle shape: (left) in water, repulsion by surface charge extends to long-range, resulting in an apparently nonchiral rod; (right) addition of NaCl decreases repulsion range and the effective particle becomes a twisted rod (Reprinted with permission from ref 105. Copyright 2001 American Chemical Society).
species to give nematic order. Its origin can be attributed to favorably excluded volume interactions leading to higher packing entropy compared with the disordered phase. The origin of this spontaneous self-assembly phenomenon was proposed to be akin to the helicoidal structures often observed in naturally occurring materials containing cellulose.114,168,169 Because of the absence of any structural chirality in the molecules in these suspensions, this helicoidal arrangement was assumed to be due to an asymmetry that induces chiral nematic packing. Revol and Marchessault hypothesized that there must be a twist in the CNs themselves that accounts for their chiral interaction.166 Thus, because suspensions of uncharged CNs, generated from HCl, do not give rise to such chiral nematic order, negative charges from ionized sulfate groups on the surface of CNs were thought to be imperative for phase stability, and their helical distribution has also been suggested to be the “twisting agent”.114 However, recent studies carried out on suspensions in which CNs were sterically stabilized by surfactant coating129 or polymer grafting127 provided more evidence of twists in the CN nanostructure. In fact, it has been found that even if electrostatic repulsions are screened after rudimentary adsorption or grafting modifications to the CNs, the suspensions conserve their chiral nematic order.127,129 Orts et al.170 have confirmed, based on in situ small angle neutron scattering (SANS) measurements of CNs in aqueous suspension (under magnetic field and shear alignment), the hypothesis that CNs are screw-like rods (Figure 12, top). More supporting evidence was reported by Araki and Kuga105 who showed that surprisingly, CNs from bacterial cellulose form a nonchiral nematic phase in an electrolyte-free suspension,
whereas in the presence of an electrolyte, the suspension assumes chiral nematic order. This phenomenon was explained by nontrivial morphological changes in the CN, that is, from a plain cylindrical configuration to a twisted rod, as a result of the screening of surface charge (Figure 12, bottom). In fact, the dilatation of CNs resulting from the repulsive force by surface charges would obscure the chiral morphology, making the effective rods straight and smooth; permitting this configuration to lead to the formation of a nematic phase by parallel packing of these rods. Addition of an electrolyte would induce shrinkage of the effective particle size; in this scenario, the twisted morphology manifests itself in mutual alignment of the rods and results in the formation of chiral nematic order (Figure 12 bottom). The concept of ordered chiral nematic phases and their properties such as those observed in CN suspensions has been shown to be dictated by classical phase equilibrium theories related to colloidal liquid crystals such as the Onsager theory171 or its extended version such as the Stroobants, Lekkerkerker, and Odijk (SLO) theory.172 The phase-forming ability depends on several parameters such as the aspect ratio of the particles, the charge density, and the osmotic pressure.
5.1. Self-Assembly and -Organization of CNs in Aqueous Medium The critical concentration of sulfated CNs necessary for the formation of ordered nematic phases in electrolyte-free aqueous suspensions depends to a large degree on the charge density and typically ranges between 1% and 10% (w/w). The resultant chiral nematic anisotropic phases typically
Chemical Reviews, 2010, Vol. 110, No. 6 3491
Figure 13. Effect of added NaCl on the phase behavior of suspensions of CNs from bacterial cellulose for a fixed total cellulose concentration of 3 wt % after 25 days of standing. Reprinted with permission from Ref 106. Copyright 2009 American Chemical Society.
Figure 14. Polarized-light micrographs of CN suspensions: (left) fingerprint pattern in the chiral nematic phase of the directly H2SO4hydrolyzed suspension (initial solid content, 5.4%); (right) crosshatch pattern of postsulfated suspension (solid content, 7.1%). Reprinted with permission from ref 86. Copyright 2000 American Chemical Society.
display a pitch that decreases with increasing CN concentration and can vary from 20 to 80 µm. The isotropic-to-anisotropic (chiral nematic phase) equilibrium is sensitive to the presence of electrolytes and the specific nature of the electrolyte counterions. Quantitative studies of the changes in composition of the isotropic and anisotropic phases as a function of electrolyte concentration where both phases coexist,128 as well as the effect of the type of counterion,173 have been conducted. It has been found from the latter study that increasing the amount of added electrolyte decreases anisotropic phase formation. Interestingly, the chiral nematic pitch was found to decrease, that is, the phase became more highly twisted, as the electrolyte concentration increased. Apparently, the decrease in pitch occurred because the decrease in the electrical double layer thickness increased the chiral interactions between the crystallites.128 As already indicated, the phase separation of sulfated CN suspensions also depends strongly on the nature of their counterions.173 For inorganic counterions, the critical concentration for ordered phase formation increases in general as a function of increasing van der Waals’ radii, in the order H+ < Na+ < K+ < Cs+. For organic counterions such as NH4+, (CH3)4N+, (CH3CH2)4N+, (CH3CH2CH2)4N+, (CH3CH2CH2CH2)4N+, (CH3)3HN+, and (CH3CH2)3HN+, the critical concentration depends on the relative contributions of hydrophobic attraction and steric repulsion. In general, most of the work in this area has demonstrated that the critical concentration increases with increasing counterion size. It was also found that the chemical nature of the counterions also influences the stability, the temperature dependence of the phase separation, the chiral nematic pitch, and the redispersibility of dried samples made from the suspensions. Sulfuric acid-hydrolyzed CNs obtained from bacterial cellulose have been reported to spontaneously separate in a nematic phase.105 This phase separation event is preceded by a birefringent glass-like state that can persist for up to 7 days. However, adding a trace electrolyte (